"The opinions, findings and conclusions expressed in this publication are
those of the authors and not necessarily those of the Florida Department of
Transportation or the U.S. Department of Transportation.
Prepared in cooperation with the State of Florida Department of
Transportation and the U.S. Department of Transportation."
TENSILE BEHAVIOR AND DESIGN OF
SINGLE ADHESIVE ANCHORS
Ronald A. Cook, P.E.
Fernando E. Fagundo, P.E.
Michael H. Biller
Daniel E. Richardson
Department of Civil Engineering
College of Engineering
University of Florida
Engineering and Industrial Experiment Station
TABLE OF CONTENTS CHAPTERS
1 INTRODUCTION...1 1.1 Problem Statement ...1 1.2 Scope and Objectives...2
1.2.1 Scope 2 1.2.2 Objectives .3
2 BACKGROUND.4 2.1 Behavior of Adhesive Anchors....4 2.2 Other Factors Affecting Adhesive Anchor Behavior...7 2.3 Current Qualification specifications....8 3 DE VELOPMENT.OF EXPERIMENTAL PROGRAM9
3.1 General....9 3.2 Test Specimens9 3.3 Test Method..10
4 IMPLEMENTATION OF TEST PROGRAM.12 4.1 Design and Construction of Concrete Test Slabs..12
4.1.1 Formwork...12 4.1.2 Test Slab.13
4.2 Anchor Installation14 4.2.1 Anchor Bolt Preparation14
4.2.2 Hole Preparation14 4.2.3 Anchor Installation.15
4.3 Test Equipment and Procedure..17 4.3.1 Confined Testing17 4.3.2 Data Acquisition..19 4.3.3 Unconfined Testing21
4.4 Test Matrix21 5 TEST RESULTS23
5.1 General..23 5.2 Failure Modes23
5.2.1 Confined Testing and Fully-Bonded Anchors...23 5.2.2 Testing with Partially-Bonded Anchors....24 5.2.3 Unconfined Testing and Fully-Bonded Anchors...26 5.3 Description of Test Data.27
6 BEHAVIORAL MODELS FOR ADHESIVE ANCHORS..29 6.1 General29 6.2 Elastic Model for Adhesive Anchors.29
6.2.1 Development of Model..29 6.2.2 Application of Model to Test Data.33
6.3 Uniform Bond Stress Model..36 6.3.1 Development of Model..36 6.3.2 Application of Model to Test Data37 6.4 Comparison of Models to Test Results.38
6.4.1 Elastic Model.38 6.4.2 Uniform Bond Stress Model..40
7 DISCUSSION OF RESULTS...45 7.1 General...45 7.2 Design Procedures.45 7.2.1 Effective Embedment Length45 7.2.2 Bond Stress Distribution46
7.2.3 Capacity Reduction Factors...46 7.3 Qualification of Products47
8 SUMMARY, CONCLUSIONS AND RECOMMENDATIONS..49 8.1 Summary49
8.2 Design Recommendations..50 8.3 Conclusions.51 8.4 Recommendations for Further Research52
A LIST OF ADHESIVES USED FOR TESTING.53
B TABULATION AND GRAPHS FOR BASELINE TEST DATA.55
C TABULATION AND GRAPHS FOR NONBASELINE TEST DATA130
D TABULATION OF EXPERIMENTALLY DETERMINED CONSTANTS144
E QUALIFICATION OF STRUCTURAL ADHESIVES..148
CHAPTER 1 INTRODUCTION
1.1 Problem Statement
The Florida Department of Transportation (FDOT) presently does not have standard
specifications for adhesive-bonded anchors in structural applications. An adhesive-
bonded anchor is a reinforcing bar or threaded rod inserted into a drilled hole in hardened
concrete with a structural adhesive acting as a bonding agent between the concrete and
the steel. Such adhesives are packaged as two component units comprised of an epoxy,
polyester, or vinylester resin and a catalyst or curing agent.
These anchors provide a viable, economical method for adding new concrete sections or
attaching steel members to existing concrete structures. Presently, most designers follow
the adhesive manufacturer's recommendations which are based on laboratory testing
specific to individual products and applications. The increasing amount of retrofit and
rehabilitation work encountered today exemplifies the need for a standard specification
for this type of anchor.
1.2 Scope and Objectives
The purpose of this project was to study the tensile behavior of adhesive-
bonded anchors when subject to static loading and to identify parameters specific to
each adhesive. Previous research (Klingner et al., 1982) has shown that if a structural
anchor has been sufficiently embedded for tension, it will also be adequate for shear.
Therefore, the tensile behavior should provide the information necessary to describe
the bond failure of an adhesive anchor.
The adhesives tested were all self-mixing and intended for structural applications. The
diameters and embedment lengths of the anchors were varied to provide a broad range of
contact surface areas and length-to-diameter ratios. The embedment lengths were chosen
as to prevent steel failure and concentrate on the bond strengths of the individual
A series of baseline tests was used to determine bond and stiffness characteristics that
are specific to each adhesive. These properties were utilized to develop a design
equation for structural adhesive anchors.
Other tests were performed to confirm the results from the baseline tests.
Experimental data will be employed to develop a qualification specification that can be
used to establish the basic parameters necessary to design a structural adhesive bonded
2.1 Behavior of Adhesive Anchors
The main- function of a structural adhesive is to transfer load from the steel anchor to
the surrounding concrete. Daws (1978) suggests four factors that contribute to the load
transfer capability of an adhesive anchor: Mechanical interlock on the adhesive-
concrete interface, chemical bond along the adhesive-concrete interface, mechanical
interlock on the adhesive-steel interface, and chemical bond along the adhesive-steel
interface. The actual failure mode of an adhesive anchor is often a combination of
mechanical interlock and chemical bond failure.
The quantity of documented research pertaining to the behavior and the bond stress
distribution of structural adhesive anchors is currently limited. One study at the
University of Texas at Austin (Collins et al., 1989) investigated the load-deflection
behavior of retrofit and cast-in-place anchors. Five-eighths inch diameter ASTM A193
Grade B7 threaded rods were installed in concrete with a specified compressive
strength of 3600 psi (actua1 4500-6750 psi). The embedment lengths ranged from 7 to
12 in. and the anchors were allowed to cure for either 7 days or 24 hours.
The adhesive anchors were subject to unconfined testing (the reaction forces were kept
away from the anchor).
During the testing, four failure modes were experienced: yield and fracture of
the steel with anchor slip, yield and fracture of the steel without anchor slip, failure of
the bond between the adhesive and the concrete, and the failure of the bond between the
adhesive and the steel.
Just before failure, the anchors apparently resisted the loading until it reached a
level of maximum bond stress. Beyond that point, the anchor and adhesive began to slip
out as a unit. Little or no anchor slip was detected before bond failure. After bond
failure, residual anchor strength was apparently due to mechanical interlock between the
adhesive and the concrete.
Failure of the bond between the adhesive and the concrete occurred at loads ranging
from about one-third of the anchor steel capacity to the full capacity of the anchor steel.
Another study at the University of Texas at Austin (Doerr et al., 1989) also investigated
the behavior of structural adhesive anchors. Data from these experiments was used to
develop a design equation that, given certain characteristics of the anchoring system,
predicts anchor capacity. Five-eighths inch diameter ASTM A193 Grade B7 threaded rods
were installed in 3600 psi concrete and subject to unconfined testing. The anchors tested
were either fully bonded (adhesive covered the entire embedded portion of anchor) or
partially bonded (top 2 in. of the embedded portion of the anchor treated with
a debonding agent) and embedment depths ranged from 4 to 8 in.
During the testing, the fully bonded anchors failed either by fracture of
the steel or by the formation of a shallow (about l to 2 in.) concrete cone
accompanied by pullout of the adhesive. The partially bonded anchors failed
either by fracture of the steel or by the pullout of an adhesive core. Concrete
cone failures did not occur with the partially bonded anchors. Test data
revealed that fully bonded anchors had only slightly higher capacities than the
partially bonded anchors of the same embedment length.
The following equation for anchor strength was found using an elastic
where Pmax is the maximum tensile force, umax is the maximum bond stress, '
is a stiffness parameter of the adhesive (exp erimentally determined), d is the
hole diameter, and is the embedment length. This model provided the best
fit for the test data.
For each adhesive, a value for umax and ' was calculated based on the
experimental results. Load resistance factors, based on the asymptotic nature
of the equation were suggested for design use.
If P is within 95% of the asymptotic value, =0.80. Otherwise, =0.60.
The study (1989b) also found that a uniform bond stress distribution serves as a
reasonable approximation of the load capacity of an adhesive anchor.
lduP maxmax =
2.2 Other Factors Affecting Adhesive Anchor Behavior
Structural adhesives are sensitive to several factors. Misproportioning the resin
and curing agent, even by a slight amount, may affect curing time and bond strength.
The wetting characteristics (ability of the adhesive to coat the entire surface of the
embedded portion of the anchor) of each adhesive affect the ability of the adhesive to
distribute bond stress to the surrounding concrete along the bonded length of the
Other factors that may affect adhesive behavior include hot temperatures often
experienced during the summer months in warmer climates, high lime concentrations,
moisture, and ultraviolet light. Testing under such conditions is beyond the scope of
this project and is recommended for further research.
2.3 Current Qualification Specifications
The Florida Department of Transportation (FDOT) does not currently have a
specification for adhesive anchors in structural applications. Section 460-30 of the
current FDOT code (1986) contains specifications pertaining to setting and furnishing
anchor bolts (i.e. bolt composition, cleaning and drilling holes, etc.). Classification of
each type of adhesive compound is listed in Section 926-1. A Type J adhesive is "an
epoxy for anchor bolts where strength of the overall structure is not a factor such as
for hanging telephone lines or other utility attachments" (1986, p. 644). Section 926-2
lists specifications for each type of adhesive and makes a reference to the FDOT
Qualified Products List (1990).
One current qualification test for structural adhesive anchors is specified by the
Missouri Highway and Transportation Department (MHTD). Section 1039.3 and T49-
2-90 in MHTD Standard Specifications (1990) specifies a pull-out test for chemical
bonding agents. Given a standardized concrete compressive strength, hole depth and
diameter, anchor diameter, anchor length, adhesive curing time, and loading rate, the
adhesive anchor must withstand a specified minimum load.
The method of testing (confined or unconfined) is not specified.
DEVELOPMENT OF EXPERIMENTAL PROGRAM
The test program consisted of baseline tests that were performed on each of 16
adhesives. The purpose of these tests was to determine bond and stiffness properties
specific to each adhesive. These characteristics were utilized to develop a design
equation for adhesive anchors. Additional tests were used to verify the results of the
3.2 Test Specimens
The structural adhesive anchors tested were ASTM A193 Grade B7 threaded rods.
The anchor diameters were , 5/8, and and their respective embedment lengths
were 5, 3.5, and 7": These combinations of dimensions were chosen to provide a wide
range in the specimens / d ratio. This relationship was determined to be important in
modeling the behavior of adhesive anchors (see Chapter 6).
High strength (minimum specified tensile strength of 125 ksi) threaded rod was used to
ensure that the bond would fail before the steel began to yield under tensile loading. The
adhesives tested are intended to be used in structural
applications. Many of the products are currently included in the FDOT Qualified
Products List (1990).
3.3 Test Methods
Static tensile tests were performed two ways--confined and unconfined. A
confined test requires that the reaction force be kept close to the anchor. An
unconfined test requires the reaction force to be kept away from the anchor. For both
testing methods, the adhesive anchors were either fully bonded or partially bonded.
The fully-bonded anchors had the adhesive over the entire embedded length of the
steel. Partially-bonded anchors were debonded at the top 2 in. of the embedded length.
The baseline tests involved confined testing with fullybonded anchors. The tests
were performed in accordance with ASTM Z1706z (1991). This method of testing
prevented spalling at the surface of the concrete. By eliminating concrete cone
formations, confined testing allowed for the study of the bond strength while
neglecting the tensile strength of the concrete.
Unconfined tests were performed in accordance with ASTM E488. Fully bonded
anchors were studied under this loading condition since it is often encountered in
many engineering applications. Since concrete cone formation is possible with
unconfined testing, concrete tensile strength may be a factor.
The results of these tests are compared with the baseline tests.
Partially bonded anchors were studied under both confined and unconfined
testing. Previous tests (Doerr et al., 1989) have shown that the depth of a typical concrete
cone formed during failure is about 2 in. To avoid cone formation, these anchors were
debonded along the top 2 in. of the embedded length. The strength of the partially-
bonded anchors were compared to that of the fully-bonded anchors of the same diameter
and embedment depth. Design equations, derived using results of the baseline tests, were
used to predict the capacity of the debonded anchors. The accuracy of the design
equation was investigated by comparing the calculated values with the actual test data.
IMPLEMENTATION OF TEST PROGRAM
4.1 Design and Construction of Concrete Test Slabs
As shown in Figure 4-1, the formwork was designed so that two slabs could be
cast at once. The center divider was permanently attached to the base. Removable side
panels were employed for both easy stripping and reuse.
Figure 4-1 Formwork with steel reinforcement